#------------------------------------------------------------------------------
#$Date: 2016-03-23 00:19:13 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179104 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/66/4306608.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4306608
loop_
_publ_author_name
'Céline Pichon'
'Pierre Mialane'
'Anne Dolbecq'
'Jérôme Marrot'
'Eric Rivière'
'Bassem S. Bassil'
'Ulrich Kortz'
'Bineta Keita'
'Louis Nadjo'
'Francis Sécheresse'
_publ_contact_author
; 
      Dr P. Mialane
      Institut Lavoisier de Versailles, UMR 8180
      Université de Versailles Saint-Quentin-en-Yvelines
      45 Avenue des Etats Unis
      78035 Versailles cedex
      France
;
_publ_contact_author_email       mialane@chimie.uvsq.fr
_publ_contact_author_fax         '(33) 1 39 25 43 81'
_publ_contact_author_phone       '(33) 1 39 25 43 83'
_publ_section_title
;
Octa- and Nonanuclear Nickel(II) Polyoxometalate Clusters: Synthesis and
Electrochemical and Magnetic Characterizations
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11120
_journal_page_last               11128
_journal_paper_doi               10.1021/ic801431f
_journal_volume                  47
_journal_year                    2008
_chemical_formula_sum            'C12 H18 N6 Na16 Ni8 O121 Si2 W18'
_chemical_formula_weight         6385.32
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           148
_symmetry_cell_setting           rhombohedral
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   11.9660(7)
_cell_length_b                   11.9660(7)
_cell_length_c                   72.753(7)
_cell_measurement_reflns_used    9102
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      30.06
_cell_measurement_theta_min      2.26
_cell_volume                     9021.5(11)
_computing_cell_refinement       'Bruker APEX2'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 512x512
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0739
_diffrn_reflns_av_sigmaI/netI    0.0252
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       102
_diffrn_reflns_limit_l_min       -102
_diffrn_reflns_number            113265
_diffrn_reflns_theta_full        30.08
_diffrn_reflns_theta_max         30.08
_diffrn_reflns_theta_min         0.84
_exptl_absorpt_coefficient_mu    18.557
_exptl_absorpt_correction_T_max  0.7079
_exptl_absorpt_correction_T_min  0.2584
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, V2.10)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    3.526
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       platelet
_exptl_crystal_F_000             8580
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.804
_refine_diff_density_min         -3.740
_refine_diff_density_rms         0.676
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.263
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         5901
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.263
_refine_ls_R_factor_all          0.0337
_refine_ls_R_factor_gt           0.0271
_refine_ls_shift/su_max          0.007
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0554P)²+131.1312P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0855
_refine_ls_wR_factor_ref         0.1012
_reflns_number_gt                5379
_reflns_number_total             5901
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801431f_si_003_2.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Rhombohedral' changed to 'rhombohedral'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               4306608
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.004464(8) 0.161073(8) 0.144517(1) 0.00970(2) Uani 1 1 d . . .
W2 W -0.184406(8) 0.156381(8) 0.101827(1) 0.01040(2) Uani 1 1 d . . .
W3 W 0.176684(8) 0.343172(8) 0.102629(1) 0.01071(2) Uani 1 1 d . . .
Ni1 Ni 0.17590(3) 0.18202(3) 0.067710(5) 0.01314(8) Uani 1 1 d . . .
Ni2 Ni 0.0000 0.0000 0.040274(8) 0.01689(13) Uani 1 3 d S . .
Si1 Si 0.0000 0.0000 0.103876(15) 0.0064(2) Uani 1 3 d S . .
O1 O -0.00021(16) 0.26774(16) 0.16086(3) 0.0154(5) Uani 1 1 d . . .
O2 O 0.12333(15) 0.27238(15) 0.12833(2) 0.0106(4) Uani 1 1 d . . .
O3 O -0.13142(15) 0.14891(15) 0.12854(2) 0.0105(4) Uani 1 1 d . . .
O4 O 0.12695(15) 0.12879(16) 0.15559(3) 0.0137(4) Uani 1 1 d . . .
O5 O 0.0000 0.0000 0.12658(4) 0.0089(6) Uani 1 3 d S . .
O6 O -0.23904(15) 0.26163(16) 0.10680(3) 0.0156(4) Uani 1 1 d . . .
O7 O -0.21690(15) 0.13244(16) 0.07767(3) 0.0155(5) Uani 1 1 d . . .
O8 O -0.00487(15) 0.27584(16) 0.09923(3) 0.0133(4) Uani 1 1 d . . .
O9 O -0.33817(15) -0.00545(15) 0.10850(3) 0.0126(4) Uani 1 1 d . . .
O10 O -0.12930(14) -0.00122(15) 0.09675(2) 0.0113(4) Uani 1 1 d . . .
O11 O 0.22537(16) 0.50047(16) 0.10855(3) 0.0159(5) Uani 1 1 d . . .
O12 O 0.20796(16) 0.35403(16) 0.07834(3) 0.0152(5) Uani 1 1 d . . .
O13 O -0.0030(2) 0.1257(2) 0.05845(4) 0.0127(5) Uani 0.67 1 d P . .
N1 N -0.0083(6) 0.1374(6) 0.05829(10) 0.0127(5) Uani 0.33 1 d P . .
N2 N -0.0143(10) 0.2235(7) 0.04992(14) 0.064(3) Uani 0.33 1 d PD . .
N3 N -0.0202(10) 0.3023(8) 0.03938(15) 0.064(3) Uani 0.33 1 d PD . .
O14 O 0.26916(19) 0.27840(19) 0.04383(3) 0.0222(6) Uani 1 1 d . . .
O15 O 0.13410(19) 0.13753(19) 0.02314(3) 0.0245(6) Uani 1 1 d . . .
C1 C 0.2345(3) 0.2406(3) 0.02744(4) 0.0239(8) Uani 1 1 d . . .
C2 C 0.3191(4) 0.3272(4) 0.01210(5) 0.0500(15) Uani 1 1 d . . .
H2A H 0.3995 0.3244 0.0116 0.075 Uiso 1 1 calc R . .
H2B H 0.3389 0.4160 0.0144 0.075 Uiso 1 1 calc R . .
H2C H 0.2737 0.2973 0.0004 0.075 Uiso 1 1 calc R . .
Na1 Na 0.6667 0.3333 0.12762(3) 0.0155(4) Uani 1 3 d S . .
Na2 Na 0.0000 0.0000 0.0000 0.0281(8) Uani 1 6 d S . .
Na3 Na 0.35003(10) 0.34869(10) 0.141853(16) 0.0203(3) Uani 1 1 d . . .
Na4 Na 0.3350(2) 0.50243(19) 0.05680(3) 0.0293(6) Uani 0.58 1 d P . .
Na5 Na -0.3401(2) 0.1623(2) 0.05656(4) 0.0203(3) Uani 0.42 1 d P . .
Na6 Na 0.3333 0.6667 0.13080(8) 0.0475(16) Uani 0.50 3 d SP . .
O1W O 0.53586(18) 0.13096(19) 0.14172(3) 0.0217(5) Uani 1 1 d . . .
O2W O 0.3333 0.6667 0.07523(6) 0.0313(10) Uani 1 3 d S . .
O3W O 0.3333 0.6667 0.1667 0.0305(14) Uani 1 6 d S . .
O4W O -0.3333 0.3333 0.07379(7) 0.0455(14) Uani 1 3 d S . .
O5W O 0.5078(3) 0.5093(3) 0.07620(5) 0.0550(11) Uani 1 1 d . . .
O6W O 0.1533(3) 0.5694(4) 0.14327(6) 0.0689(12) Uani 1 1 d . . .
O7W O 0.3333 0.6667 0.00010(13) 0.041(2) Uani 0.50 3 d SP . .
O8W O 0.1936(6) 0.5273(5) 0.03652(9) 0.0567(19) Uani 0.50 1 d P . .
O9W O 0.2169(6) 0.7298(5) 0.15233(10) 0.055(2) Uani 0.50 1 d P . .
O10W O 0.1242(7) 0.4524(8) 0.0407(2) 0.116(5) Uani 0.50 1 d P . .
O11W O -0.1910(11) 0.3264(8) 0.03667(13) 0.069(3) Uani 0.33 1 d P . .
O12W O -0.1266(9) 0.3147(8) 0.0410(2) 0.080(5) Uani 0.33 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O3 102.08(9) . . ?
O1 W1 O2 101.34(8) . . ?
O3 W1 O2 90.42(7) . . ?
O1 W1 O4 100.44(8) . 2 ?
O3 W1 O4 89.71(7) . 2 ?
O2 W1 O4 157.69(8) . 2 ?
O1 W1 O4 97.59(9) . . ?
O3 W1 O4 160.28(8) . . ?
O2 W1 O4 87.03(8) . . ?
O4 W1 O4 85.37(9) 2 . ?
O1 W1 O5 169.85(9) . . ?
O3 W1 O5 86.64(7) . . ?
O2 W1 O5 83.58(7) . . ?
O4 W1 O5 74.15(7) 2 . ?
O4 W1 O5 73.64(7) . . ?
O1 W1 Na3 91.88(6) . 2 ?
O3 W1 Na3 41.13(5) . 2 ?
O2 W1 Na3 131.54(6) . 2 ?
O4 W1 Na3 52.09(5) 2 2 ?
O4 W1 Na3 137.45(5) . 2 ?
O5 W1 Na3 91.38(2) . 2 ?
O1 W1 Na3 89.22(6) . . ?
O3 W1 Na3 131.45(5) . . ?
O2 W1 Na3 41.06(6) . . ?
O4 W1 Na3 134.89(5) 2 . ?
O4 W1 Na3 49.57(5) . . ?
O5 W1 Na3 88.81(2) . . ?
Na3 W1 Na3 172.51(3) 2 . ?
O6 W2 O7 101.05(10) . . ?
O6 W2 O8 99.80(8) . . ?
O7 W2 O8 95.51(7) . . ?
O6 W2 O9 99.15(8) . . ?
O7 W2 O9 93.66(7) . . ?
O8 W2 O9 156.93(9) . . ?
O6 W2 O3 94.07(9) . . ?
O7 W2 O3 164.86(9) . . ?
O8 W2 O3 82.53(7) . . ?
O9 W2 O3 83.12(7) . . ?
O6 W2 O10 174.11(6) . . ?
O7 W2 O10 80.84(8) . . ?
O8 W2 O10 85.51(7) . . ?
O9 W2 O10 75.10(7) . . ?
O3 W2 O10 84.04(7) . . ?
O6 W2 Na3 83.93(6) . 2 ?
O7 W2 Na3 135.65(5) . 2 ?
O8 W2 Na3 127.39(6) . 2 ?
O9 W2 Na3 42.49(6) . 2 ?
O3 W2 Na3 44.96(4) . 2 ?
O10 W2 Na3 90.82(5) . 2 ?
O11 W3 O12 102.85(9) . . ?
O11 W3 O8 100.62(9) . . ?
O12 W3 O8 93.14(8) . . ?
O11 W3 O9 99.97(8) . 3 ?
O12 W3 O9 92.84(9) . 3 ?
O8 W3 O9 156.68(7) . 3 ?
O11 W3 O2 95.16(8) . . ?
O12 W3 O2 162.00(8) . . ?
O8 W3 O2 83.63(7) . . ?
O9 W3 O2 83.73(8) 3 . ?
O11 W3 O10 173.61(8) . 3 ?
O12 W3 O10 80.20(7) . 3 ?
O8 W3 O10 84.72(8) . 3 ?
O9 W3 O10 74.14(7) 3 3 ?
O2 W3 O10 81.86(7) . 3 ?
O11 W3 Na3 84.39(7) . . ?
O12 W3 Na3 134.29(7) . . ?
O8 W3 Na3 130.35(6) . . ?
O9 W3 Na3 41.81(6) 3 . ?
O2 W3 Na3 46.77(5) . . ?
O10 W3 Na3 89.47(5) 3 . ?
O13 Ni1 N1 85.9(2) . 3 ?
O13 Ni1 O7 173.31(9) . 3 ?
N1 Ni1 O7 88.4(2) 3 3 ?
O13 Ni1 O13 81.22(17) . 3 ?
N1 Ni1 O13 5.1(3) 3 3 ?
O7 Ni1 O13 92.98(10) 3 3 ?
O13 Ni1 O12 95.55(10) . . ?
N1 Ni1 O12 177.3(2) 3 . ?
O7 Ni1 O12 90.00(7) 3 . ?
O13 Ni1 O12 174.77(10) 3 . ?
O13 Ni1 O14 95.30(10) . . ?
N1 Ni1 O14 93.3(2) 3 . ?
O7 Ni1 O14 88.53(9) 3 . ?
O13 Ni1 O14 95.56(10) 3 . ?
O12 Ni1 O14 88.81(8) . . ?
O13 Ni1 N1 4.3(2) . . ?
N1 Ni1 N1 90.2(4) 3 . ?
O7 Ni1 N1 177.02(19) 3 . ?
O13 Ni1 N1 85.5(2) 3 . ?
O12 Ni1 N1 91.4(2) . . ?
O14 Ni1 N1 94.1(2) . . ?
O13 Ni1 O10 98.33(9) . 3 ?
N1 Ni1 O10 98.2(2) 3 3 ?
O7 Ni1 O10 78.98(8) 3 3 ?
O13 Ni1 O10 96.92(9) 3 3 ?
O12 Ni1 O10 79.42(6) . 3 ?
O14 Ni1 O10 162.75(7) . 3 ?
N1 Ni1 O10 98.7(2) . 3 ?
O13 Ni1 Ni2 43.43(9) . . ?
N1 Ni1 Ni2 47.0(2) 3 . ?
O7 Ni1 Ni2 132.50(5) 3 . ?
O13 Ni1 Ni2 43.46(8) 3 . ?
O12 Ni1 Ni2 135.15(6) . . ?
O14 Ni1 Ni2 80.18(5) . . ?
N1 Ni1 Ni2 47.0(2) . . ?
O10 Ni1 Ni2 117.05(5) 3 . ?
O13 Ni1 Na4 101.60(9) . . ?
N1 Ni1 Na4 141.3(2) 3 . ?
O7 Ni1 Na4 85.05(6) 3 . ?
O13 Ni1 Na4 144.07(9) 3 . ?
O12 Ni1 Na4 40.52(7) . . ?
O14 Ni1 Na4 48.58(7) . . ?
N1 Ni1 Na4 97.71(19) . . ?
O10 Ni1 Na4 117.70(6) 3 . ?
Ni2 Ni1 Na4 117.82(4) . . ?
O13 Ni1 Na5 145.23(9) . 3 ?
N1 Ni1 Na5 93.1(2) 3 3 ?
O7 Ni1 Na5 38.63(7) 3 3 ?
O13 Ni1 Na5 98.08(10) 3 3 ?
O12 Ni1 Na5 86.93(6) . 3 ?
O14 Ni1 Na5 50.00(8) . 3 ?
N1 Ni1 Na5 144.10(19) . 3 ?
O10 Ni1 Na5 116.14(7) 3 3 ?
Ni2 Ni1 Na5 116.08(5) . 3 ?
Na4 Ni1 Na5 59.42(6) . 3 ?
O13 Ni2 O13 81.64(12) 3 2 ?
O13 Ni2 O13 81.64(12) 3 . ?
O13 Ni2 O13 81.64(12) 2 . ?
O13 Ni2 O15 95.77(11) 3 . ?
O13 Ni2 O15 176.50(10) 2 . ?
O13 Ni2 O15 95.68(9) . . ?
O13 Ni2 O15 95.69(9) 3 3 ?
O13 Ni2 O15 95.78(11) 2 3 ?
O13 Ni2 O15 176.50(10) . 3 ?
O15 Ni2 O15 86.81(8) . 3 ?
O13 Ni2 O15 176.50(10) 3 2 ?
O13 Ni2 O15 95.68(9) 2 2 ?
O13 Ni2 O15 95.78(11) . 2 ?
O15 Ni2 O15 86.81(8) . 2 ?
O15 Ni2 O15 86.80(8) 3 2 ?
O13 Ni2 N1 3.6(2) 3 3 ?
O13 Ni2 N1 85.0(2) 2 3 ?
O13 Ni2 N1 83.20(18) . 3 ?
O15 Ni2 N1 92.4(2) . 3 ?
O15 Ni2 N1 94.25(17) 3 3 ?
O15 Ni2 N1 178.67(18) 2 3 ?
O13 Ni2 N1 85.0(2) 3 . ?
O13 Ni2 N1 83.21(18) 2 . ?
O13 Ni2 N1 3.6(2) . . ?
O15 Ni2 N1 94.25(17) . . ?
O15 Ni2 N1 178.67(18) 3 . ?
O15 Ni2 N1 92.4(2) 2 . ?
N1 Ni2 N1 86.5(3) 3 . ?
O13 Ni2 N1 83.21(18) 3 2 ?
O13 Ni2 N1 3.6(2) 2 2 ?
O13 Ni2 N1 85.0(2) . 2 ?
O15 Ni2 N1 178.67(18) . 2 ?
O15 Ni2 N1 92.4(2) 3 2 ?
O15 Ni2 N1 94.25(17) 2 2 ?
N1 Ni2 N1 86.5(3) 3 2 ?
N1 Ni2 N1 86.5(3) . 2 ?
O13 Ni2 Ni1 44.04(6) 3 . ?
O13 Ni2 Ni1 96.03(9) 2 . ?
O13 Ni2 Ni1 43.31(8) . . ?
O15 Ni2 Ni1 80.47(6) . . ?
O15 Ni2 Ni1 135.16(7) 3 . ?
O15 Ni2 Ni1 134.53(7) 2 . ?
N1 Ni2 Ni1 44.20(15) 3 . ?
N1 Ni2 Ni1 45.93(19) . . ?
N1 Ni2 Ni1 99.3(2) 2 . ?
O13 Ni2 Ni1 43.31(8) 3 3 ?
O13 Ni2 Ni1 44.04(6) 2 3 ?
O13 Ni2 Ni1 96.03(9) . 3 ?
O15 Ni2 Ni1 134.53(7) . 3 ?
O15 Ni2 Ni1 80.47(6) 3 3 ?
O15 Ni2 Ni1 135.16(7) 2 3 ?
N1 Ni2 Ni1 45.93(19) 3 3 ?
N1 Ni2 Ni1 99.3(2) . 3 ?
N1 Ni2 Ni1 44.21(15) 2 3 ?
Ni1 Ni2 Ni1 78.636(17) . 3 ?
O13 Ni2 Ni1 96.03(9) 3 2 ?
O13 Ni2 Ni1 43.31(8) 2 2 ?
O13 Ni2 Ni1 44.04(6) . 2 ?
O15 Ni2 Ni1 135.15(7) . 2 ?
O15 Ni2 Ni1 134.53(7) 3 2 ?
O15 Ni2 Ni1 80.47(6) 2 2 ?
N1 Ni2 Ni1 99.3(2) 3 2 ?
N1 Ni2 Ni1 44.20(15) . 2 ?
N1 Ni2 Ni1 45.93(19) 2 2 ?
Ni1 Ni2 Ni1 78.636(16) . 2 ?
Ni1 Ni2 Ni1 78.636(16) 3 2 ?
O10 Si1 O10 110.32(7) 2 3 ?
O10 Si1 O10 110.32(7) 2 . ?
O10 Si1 O10 110.32(7) 3 . ?
O10 Si1 O5 108.61(7) 2 . ?
O10 Si1 O5 108.61(7) 3 . ?
O10 Si1 O5 108.61(7) . . ?
W1 O1 Na3 150.34(12) . 14_455 ?
W1 O2 W3 149.34(9) . . ?
W1 O2 Na3 110.72(8) . . ?
W3 O2 Na3 98.53(6) . . ?
W1 O3 W2 147.49(10) . . ?
W1 O3 Na3 109.51(8) . 2 ?
W2 O3 Na3 99.36(7) . 2 ?
W1 O4 W1 120.01(9) 3 . ?
W1 O4 Na3 95.21(7) 3 . ?
W1 O4 Na3 98.48(7) . . ?
Si1 O5 W1 123.72(6) . 3 ?
Si1 O5 W1 123.72(6) . 2 ?
W1 O5 W1 92.16(8) 3 2 ?
Si1 O5 W1 123.72(6) . . ?
W1 O5 W1 92.16(8) 3 . ?
W1 O5 W1 92.16(8) 2 . ?
W2 O6 Na1 148.08(11) . 1_455 ?
W2 O7 Ni1 111.30(11) . 2 ?
W2 O7 Na5 137.91(14) . . ?
Ni1 O7 Na5 107.47(11) 2 . ?
W2 O8 W3 156.72(12) . . ?
W3 O9 W2 118.37(10) 2 . ?
W3 O9 Na3 105.99(9) 2 2 ?
W2 O9 Na3 104.71(7) . 2 ?
Si1 O10 Ni1 124.51(11) . 2 ?
Si1 O10 W2 126.79(8) . . ?
Ni1 O10 W2 88.87(7) 2 . ?
Si1 O10 W3 125.29(10) . 2 ?
Ni1 O10 W3 88.59(5) 2 2 ?
W2 O10 W3 91.28(7) . 2 ?
W3 O11 Na6 145.85(14) . . ?
W3 O12 Ni1 111.79(9) . . ?
W3 O12 Na4 139.82(10) . . ?
Ni1 O12 Na4 103.87(10) . . ?
N2 O13 Ni1 113.7(4) . . ?
N2 O13 Ni2 112.4(5) . . ?
Ni1 O13 Ni2 93.27(13) . . ?
N2 O13 Ni1 107.0(5) . 2 ?
Ni1 O13 Ni1 132.82(15) . 2 ?
Ni2 O13 Ni1 92.50(9) . 2 ?
N2 N1 Ni1 114.2(7) . 2 ?
N2 N1 Ni1 116.1(6) . . ?
Ni1 N1 Ni1 126.9(4) 2 . ?
N2 N1 Ni2 112.6(7) . . ?
Ni1 N1 Ni2 88.8(2) 2 . ?
Ni1 N1 Ni2 87.1(3) . . ?
N1 N2 N3 171.7(12) . . ?
N1 N2 O13 3.7(4) . . ?
N3 N2 O13 168.4(11) . . ?
N2 N3 O12W 116.1(11) . . ?
N2 N3 O10W 109.8(9) . . ?
O12W N3 O10W 112.2(8) . . ?
C1 O14 Ni1 126.83(16) . . ?
C1 O14 Na4 126.3(2) . . ?
Ni1 O14 Na4 94.09(9) . . ?
C1 O14 Na5 122.3(2) . 3 ?
Ni1 O14 Na5 93.47(10) . 3 ?
Na4 O14 Na5 81.43(9) . 3 ?
C1 O15 Ni2 128.10(19) . . ?
C1 O15 Na2 148.41(19) . . ?
Ni2 O15 Na2 83.49(6) . . ?
O15 C1 O14 124.4(2) . . ?
O15 C1 C2 118.2(3) . . ?
O14 C1 C2 117.4(2) . . ?
C1 C2 H2A 109.5 . . ?
C1 C2 H2B 109.5 . . ?
H2A C2 H2B 109.5 . . ?
C1 C2 H2C 109.5 . . ?
H2A C2 H2C 109.5 . . ?
H2B C2 H2C 109.5 . . ?
O6 Na1 O6 81.21(10) 1_655 3 ?
O6 Na1 O6 81.21(10) 1_655 2_665 ?
O6 Na1 O6 81.21(10) 3 2_665 ?
O6 Na1 O1W 79.38(7) 1_655 2_655 ?
O6 Na1 O1W 160.59(9) 3 2_655 ?
O6 Na1 O1W 95.80(7) 2_665 2_655 ?
O6 Na1 O1W 95.80(7) 1_655 . ?
O6 Na1 O1W 79.38(7) 3 . ?
O6 Na1 O1W 160.59(9) 2_665 . ?
O1W Na1 O1W 102.53(8) 2_655 . ?
O6 Na1 O1W 160.59(9) 1_655 3_665 ?
O6 Na1 O1W 95.80(7) 3 3_665 ?
O6 Na1 O1W 79.38(7) 2_665 3_665 ?
O1W Na1 O1W 102.53(8) 2_655 3_665 ?
O1W Na1 O1W 102.53(8) . 3_665 ?
O6 Na1 Na3 65.72(5) 1_655 2_655 ?
O6 Na1 Na3 94.78(4) 3 2_655 ?
O6 Na1 Na3 146.89(7) 2_665 2_655 ?
O1W Na1 Na3 77.20(7) 2_655 2_655 ?
O1W Na1 Na3 36.42(6) . 2_655 ?
O1W Na1 Na3 133.68(8) 3_665 2_655 ?
O6 Na1 Na3 94.78(4) 1_655 3_665 ?
O6 Na1 Na3 146.88(7) 3 3_665 ?
O6 Na1 Na3 65.72(5) 2_665 3_665 ?
O1W Na1 Na3 36.42(6) 2_655 3_665 ?
O1W Na1 Na3 133.68(8) . 3_665 ?
O1W Na1 Na3 77.19(7) 3_665 3_665 ?
Na3 Na1 Na3 113.61(3) 2_655 3_665 ?
O6 Na1 Na3 146.88(7) 1_655 . ?
O6 Na1 Na3 65.72(5) 3 . ?
O6 Na1 Na3 94.78(4) 2_665 . ?
O1W Na1 Na3 133.68(8) 2_655 . ?
O1W Na1 Na3 77.20(7) . . ?
O1W Na1 Na3 36.42(6) 3_665 . ?
Na3 Na1 Na3 113.61(3) 2_655 . ?
Na3 Na1 Na3 113.61(3) 3_665 . ?
O15 Na2 O15 106.02(7) 3 11 ?
O15 Na2 O15 106.02(7) 3 10 ?
O15 Na2 O15 73.98(7) 11 10 ?
O15 Na2 O15 180.0 3 12 ?
O15 Na2 O15 73.98(7) 11 12 ?
O15 Na2 O15 73.98(7) 10 12 ?
O15 Na2 O15 73.98(7) 3 2 ?
O15 Na2 O15 180.0 11 2 ?
O15 Na2 O15 106.02(7) 10 2 ?
O15 Na2 O15 106.02(7) 12 2 ?
O15 Na2 O15 73.97(7) 3 . ?
O15 Na2 O15 106.03(7) 11 . ?
O15 Na2 O15 180.0 10 . ?
O15 Na2 O15 106.03(7) 12 . ?
O15 Na2 O15 73.97(7) 2 . ?
O15 Na2 Ni2 44.00(5) 3 . ?
O15 Na2 Ni2 135.99(5) 11 . ?
O15 Na2 Ni2 135.99(5) 10 . ?
O15 Na2 Ni2 135.99(5) 12 . ?
O15 Na2 Ni2 44.01(5) 2 . ?
O15 Na2 Ni2 44.00(5) . . ?
O15 Na2 Ni2 136.00(5) 3 10 ?
O15 Na2 Ni2 44.01(5) 11 10 ?
O15 Na2 Ni2 44.01(5) 10 10 ?
O15 Na2 Ni2 44.01(5) 12 10 ?
O15 Na2 Ni2 135.99(5) 2 10 ?
O15 Na2 Ni2 136.00(5) . 10 ?
Ni2 Na2 Ni2 180.0 . 10 ?
O1 Na3 O9W 87.33(18) 15 2_665 ?
O1 Na3 O9 165.03(9) 15 3 ?
O9W Na3 O9 107.34(18) 2_665 3 ?
O1 Na3 O6W 94.59(11) 15 2_665 ?
O9W Na3 O6W 43.11(18) 2_665 2_665 ?
O9 Na3 O6W 94.30(11) 3 2_665 ?
O1 Na3 O3 104.73(7) 15 3 ?
O9W Na3 O3 142.89(17) 2_665 3 ?
O9 Na3 O3 65.38(6) 3 3 ?
O6W Na3 O3 159.50(11) 2_665 3 ?
O1 Na3 O1W 77.33(8) 15 3_665 ?
O9W Na3 O1W 111.91(17) 2_665 3_665 ?
O9 Na3 O1W 94.00(8) 3 3_665 ?
O6W Na3 O1W 72.25(8) 2_665 3_665 ?
O3 Na3 O1W 104.99(8) 3 3_665 ?
O1 Na3 O2 126.50(8) 15 . ?
O9W Na3 O2 69.95(17) 2_665 . ?
O9 Na3 O2 63.59(7) 3 . ?
O6W Na3 O2 99.23(10) 2_665 . ?
O3 Na3 O2 74.88(7) 3 . ?
O1W Na3 O2 155.86(8) 3_665 . ?
O1 Na3 O4 75.28(7) 15 . ?
O9W Na3 O4 90.79(18) 2_665 . ?
O9 Na3 O4 106.71(7) 3 . ?
O6W Na3 O4 133.68(10) 2_665 . ?
O3 Na3 O4 60.01(6) 3 . ?
O1W Na3 O4 143.29(8) 3_665 . ?
O2 Na3 O4 58.07(6) . . ?
O1 Na3 W2 133.76(6) 15 3 ?
O9W Na3 W2 137.72(17) 2_665 3 ?
O9 Na3 W2 32.80(4) 3 3 ?
O6W Na3 W2 124.05(10) 2_665 3 ?
O3 Na3 W2 35.69(4) 3 3 ?
O1W Na3 W2 90.35(6) 3_665 3 ?
O2 Na3 W2 75.58(5) . 3 ?
O4 Na3 W2 91.23(5) . 3 ?
O1 Na3 W3 160.68(7) 15 . ?
O9W Na3 W3 80.60(17) 2_665 . ?
O9 Na3 W3 32.20(5) 3 . ?
O6W Na3 W3 86.89(9) 2_665 . ?
O3 Na3 W3 77.18(5) 3 . ?
O1W Na3 W3 121.19(6) 3_665 . ?
O2 Na3 W3 34.71(4) . . ?
O4 Na3 W3 89.76(5) . . ?
W2 Na3 W3 57.181(18) 3 . ?
O1 Na3 W1 83.76(5) 15 3 ?
O9W Na3 W1 123.07(17) 2_665 3 ?
O9 Na3 W1 90.39(5) 3 3 ?
O6W Na3 W1 166.18(9) 2_665 3 ?
O3 Na3 W1 29.36(4) 3 3 ?
O1W Na3 W1 120.43(6) 3_665 3 ?
O2 Na3 W1 71.29(4) . 3 ?
O4 Na3 W1 32.70(4) . 3 ?
W2 Na3 W1 64.414(19) 3 3 ?
W3 Na3 W1 90.21(2) . 3 ?
O1 Na3 W1 99.13(6) 15 . ?
O9W Na3 W1 70.80(16) 2_665 . ?
O9 Na3 W1 88.78(6) 3 . ?
O6W Na3 W1 111.44(8) 2_665 . ?
O3 Na3 W1 72.66(5) 3 . ?
O1W Na3 W1 175.24(6) 3_665 . ?
O2 Na3 W1 28.22(4) . . ?
O4 Na3 W1 31.95(4) . . ?
W2 Na3 W1 89.89(2) 3 . ?
W3 Na3 W1 62.692(18) . . ?
W1 Na3 W1 55.600(13) 3 . ?
O12 Na4 O8W 175.6(2) . 2_665 ?
O12 Na4 O8W 106.56(17) . . ?
O8W Na4 O8W 75.6(3) 2_665 . ?
O12 Na4 O2W 88.78(12) . . ?
O8W Na4 O2W 87.5(2) 2_665 . ?
O8W Na4 O2W 86.9(2) . . ?
O12 Na4 O5W 81.64(12) . . ?
O8W Na4 O5W 96.02(17) 2_665 . ?
O8W Na4 O5W 171.22(16) . . ?
O2W Na4 O5W 90.18(13) . . ?
O12 Na4 O10W 86.4(3) . . ?
O8W Na4 O10W 96.1(3) 2_665 . ?
O8W Na4 O10W 21.0(3) . . ?
O2W Na4 O10W 92.1(3) . . ?
O5W Na4 O10W 167.8(3) . . ?
O12 Na4 O14 72.72(9) . . ?
O8W Na4 O14 111.2(2) 2_665 . ?
O8W Na4 O14 92.08(17) . . ?
O2W Na4 O14 160.39(11) . . ?
O5W Na4 O14 93.41(13) . . ?
O10W Na4 O14 80.6(2) . . ?
O12 Na4 O10W 157.5(3) . 2_665 ?
O8W Na4 O10W 20.5(3) 2_665 2_665 ?
O8W Na4 O10W 95.9(3) . 2_665 ?
O2W Na4 O10W 91.1(3) . 2_665 ?
O5W Na4 O10W 75.8(3) . 2_665 ?
O10W Na4 O10W 116.1(5) . 2_665 ?
O14 Na4 O10W 108.5(3) . 2_665 ?
O12 Na4 Ni1 35.61(6) . . ?
O8W Na4 Ni1 148.1(2) 2_665 . ?
O8W Na4 Ni1 104.66(14) . . ?
O2W Na4 Ni1 124.38(10) . . ?
O5W Na4 Ni1 83.81(9) . . ?
O10W Na4 Ni1 85.0(2) . . ?
O14 Na4 Ni1 37.33(5) . . ?
O10W Na4 Ni1 139.2(2) 2_665 . ?
O12 Na4 Na5 85.01(11) . 3 ?
O8W Na4 Na5 96.05(17) 2_665 3 ?
O8W Na4 Na5 136.5(2) . 3 ?
O2W Na4 Na5 136.00(12) . 3 ?
O5W Na4 Na5 45.82(11) . 3 ?
O10W Na4 Na5 130.7(3) . 3 ?
O14 Na4 Na5 50.61(9) . 3 ?
O10W Na4 Na5 79.51(19) 2_665 3 ?
Ni1 Na4 Na5 61.25(7) . 3 ?
O12 Na4 Na4 132.12(8) . 2_665 ?
O8W Na4 Na4 43.85(18) 2_665 2_665 ?
O8W Na4 Na4 83.39(14) . 2_665 ?
O2W Na4 Na4 44.22(7) . 2_665 ?
O5W Na4 Na4 88.75(10) . 2_665 ?
O10W Na4 Na4 101.2(2) . 2_665 ?
O14 Na4 Na4 155.02(8) . 2_665 ?
O10W Na4 Na4 48.1(2) 2_665 2_665 ?
Ni1 Na4 Na4 166.55(4) . 2_665 ?
Na5 Na4 Na4 119.98(10) 3 2_665 ?
O12 Na4 Na4 95.21(12) . 3_565 ?
O8W Na4 Na4 83.75(15) 2_665 3_565 ?
O8W Na4 Na4 43.26(18) . 3_565 ?
O2W Na4 Na4 44.22(7) . 3_565 ?
O5W Na4 Na4 134.40(10) . 3_565 ?
O10W Na4 Na4 49.1(3) . 3_565 ?
O14 Na4 Na4 129.27(12) . 3_565 ?
O10W Na4 Na4 100.34(18) 2_665 3_565 ?
Ni1 Na4 Na4 118.85(10) . 3_565 ?
Na5 Na4 Na4 179.71(6) 3 3_565 ?
Na4 Na4 Na4 60.0 2_665 3_565 ?
O7 Na5 O4W 91.92(14) . . ?
O7 Na5 O11W 105.3(3) . . ?
O4W Na5 O11W 85.4(3) . . ?
O7 Na5 O11W 174.8(3) . 3_455 ?
O4W Na5 O11W 85.1(3) . 3_455 ?
O11W Na5 O11W 78.8(6) . 3_455 ?
O7 Na5 O5W 79.76(12) . 2 ?
O4W Na5 O5W 92.32(15) . 2 ?
O11W Na5 O5W 174.5(4) . 2 ?
O11W Na5 O5W 96.0(3) 3_455 2 ?
O7 Na5 O12W 85.1(3) . . ?
O4W Na5 O12W 91.6(3) . . ?
O11W Na5 O12W 20.9(4) . . ?
O11W Na5 O12W 99.3(5) 3_455 . ?
O5W Na5 O12W 164.5(4) 2 . ?
O7 Na5 O14 70.36(11) . 2 ?
O4W Na5 O14 160.96(14) . 2 ?
O11W Na5 O14 92.4(3) . 2 ?
O11W Na5 O14 113.1(2) 3_455 2 ?
O5W Na5 O14 91.31(12) 2 2 ?
O12W Na5 O14 80.3(3) . 2 ?
O7 Na5 O12W 156.3(3) . 3_455 ?
O4W Na5 O12W 88.3(3) . 3_455 ?
O11W Na5 O12W 98.3(5) . 3_455 ?
O11W Na5 O12W 19.6(4) 3_455 3_455 ?
O5W Na5 O12W 76.6(3) 2 3_455 ?
O12W Na5 O12W 118.5(6) . 3_455 ?
O14 Na5 O12W 110.8(3) 2 3_455 ?
O7 Na5 Na4 81.61(10) . 2 ?
O4W Na5 Na4 138.58(13) . 2 ?
O11W Na5 Na4 135.8(3) . 2 ?
O11W Na5 Na4 97.8(3) 3_455 2 ?
O5W Na5 Na4 46.26(10) 2 2 ?
O12W Na5 Na4 128.1(3) . 2 ?
O14 Na5 Na4 47.96(7) 2 2 ?
O12W Na5 Na4 82.66(19) 3_455 2 ?
O7 Na5 Na5 96.33(9) . 2_565 ?
O4W Na5 Na5 42.73(9) . 2_565 ?
O11W Na5 Na5 43.3(3) . 2_565 ?
O11W Na5 Na5 84.4(3) 3_455 2_565 ?
O5W Na5 Na5 134.97(12) 2 2_565 ?
O12W Na5 Na5 50.0(3) . 2_565 ?
O14 Na5 Na5 129.93(11) 2 2_565 ?
O12W Na5 Na5 99.8(2) 3_455 2_565 ?
Na4 Na5 Na5 177.45(12) 2 2_565 ?
O7 Na5 Na5 133.43(9) . 3_455 ?
O4W Na5 Na5 42.73(9) . 3_455 ?
O11W Na5 Na5 84.6(3) . 3_455 ?
O11W Na5 Na5 42.9(2) 3_455 3_455 ?
O5W Na5 Na5 90.34(14) 2 3_455 ?
O12W Na5 Na5 102.6(3) . 3_455 ?
O14 Na5 Na5 155.94(9) 2 3_455 ?
O12W Na5 Na5 46.6(2) 3_455 3_455 ?
Na4 Na5 Na5 122.53(12) 2 3_455 ?
Na5 Na5 Na5 60.0 2_565 3_455 ?
O7 Na5 Ni1 33.90(7) . 2 ?
O4W Na5 Ni1 125.72(13) . 2 ?
O11W Na5 Ni1 102.7(3) . 2 ?
O11W Na5 Ni1 149.1(3) 3_455 2 ?
O5W Na5 Ni1 82.64(10) 2 2 ?
O12W Na5 Ni1 82.9(3) . 2 ?
O14 Na5 Ni1 36.54(6) 2 2 ?
O12W Na5 Ni1 140.9(2) 3_455 2 ?
Na4 Na5 Ni1 59.32(6) 2 2 ?
Na5 Na5 Ni1 118.16(9) 2_565 2 ?
Na5 Na5 Ni1 166.49(5) 3_455 2 ?
O6W Na6 O6W 102.3(2) 2_665 3_565 ?
O6W Na6 O6W 102.3(2) 2_665 . ?
O6W Na6 O6W 102.3(2) 3_565 . ?
O6W Na6 O11 95.63(15) 2_665 . ?
O6W Na6 O11 160.3(2) 3_565 . ?
O6W Na6 O11 81.46(12) . . ?
O6W Na6 O11 81.46(12) 2_665 2_665 ?
O6W Na6 O11 95.63(15) 3_565 2_665 ?
O6W Na6 O11 160.3(2) . 2_665 ?
O11 Na6 O11 78.91(17) . 2_665 ?
O6W Na6 O11 160.3(2) 2_665 3_565 ?
O6W Na6 O11 81.45(12) 3_565 3_565 ?
O6W Na6 O11 95.63(14) . 3_565 ?
O11 Na6 O11 78.91(17) . 3_565 ?
O11 Na6 O11 78.91(17) 2_665 3_565 ?
O6W Na6 O9W 45.87(18) 2_665 2_665 ?
O6W Na6 O9W 114.0(3) 3_565 2_665 ?
O6W Na6 O9W 56.7(2) . 2_665 ?
O11 Na6 O9W 84.37(18) . 2_665 ?
O11 Na6 O9W 122.45(14) 2_665 2_665 ?
O11 Na6 O9W 149.71(14) 3_565 2_665 ?
O6W Na6 O9W 56.7(2) 2_665 3_565 ?
O6W Na6 O9W 45.87(18) 3_565 3_565 ?
O6W Na6 O9W 114.0(3) . 3_565 ?
O11 Na6 O9W 149.71(14) . 3_565 ?
O11 Na6 O9W 84.38(18) 2_665 3_565 ?
O11 Na6 O9W 122.45(14) 3_565 3_565 ?
O9W Na6 O9W 83.6(3) 2_665 3_565 ?
O6W Na6 O9W 114.0(3) 2_665 . ?
O6W Na6 O9W 56.7(2) 3_565 . ?
O6W Na6 O9W 45.87(18) . . ?
O11 Na6 O9W 122.45(14) . . ?
O11 Na6 O9W 149.71(14) 2_665 . ?
O11 Na6 O9W 84.37(18) 3_565 . ?
O9W Na6 O9W 83.6(3) 2_665 . ?
O9W Na6 O9W 83.6(3) 3_565 . ?
O6W Na6 O3W 64.08(18) 2_665 . ?
O6W Na6 O3W 64.08(18) 3_565 . ?
O6W Na6 O3W 64.08(18) . . ?
O11 Na6 O3W 132.80(11) . . ?
O11 Na6 O3W 132.80(11) 2_665 . ?
O11 Na6 O3W 132.80(11) 3_565 . ?
O9W Na6 O3W 50.3(2) 2_665 . ?
O9W Na6 O3W 50.3(2) 3_565 . ?
O9W Na6 O3W 50.3(2) . . ?
O6W Na6 Na3 31.78(13) 2_665 . ?
O6W Na6 Na3 132.5(2) 3_565 . ?
O6W Na6 Na3 84.84(14) . . ?
O11 Na6 Na3 66.78(5) . . ?
O11 Na6 Na3 89.05(6) 2_665 . ?
O11 Na6 Na3 145.26(17) 3_565 . ?
O9W Na6 Na3 34.57(15) 2_665 . ?
O9W Na6 Na3 88.03(14) 3_565 . ?
O9W Na6 Na3 118.1(2) . . ?
O3W Na6 Na3 78.37(9) . . ?
O6W Na6 Na3 84.84(14) 2_665 2_665 ?
O6W Na6 Na3 31.78(13) 3_565 2_665 ?
O6W Na6 Na3 132.5(2) . 2_665 ?
O11 Na6 Na3 145.26(17) . 2_665 ?
O11 Na6 Na3 66.78(5) 2_665 2_665 ?
O11 Na6 Na3 89.05(6) 3_565 2_665 ?
O9W Na6 Na3 118.1(2) 2_665 2_665 ?
O9W Na6 Na3 34.57(15) 3_565 2_665 ?
O9W Na6 Na3 88.03(14) . 2_665 ?
O3W Na6 Na3 78.37(9) . 2_665 ?
Na3 Na6 Na3 116.04(6) . 2_665 ?
Na1 O1W Na3 110.10(9) . 2_655 ?
Na4 O2W Na4 91.55(14) 2_665 3_565 ?
Na4 O2W Na4 91.55(14) 2_665 . ?
Na4 O2W Na4 91.55(14) 3_565 . ?
Na6 O3W Na6 180.0 . 13_565 ?
Na5 O4W Na5 94.55(17) 2_565 . ?
Na5 O4W Na5 94.55(17) 2_565 3_455 ?
Na5 O4W Na5 94.55(17) . 3_455 ?
Na5 O5W Na4 87.92(15) 3 . ?
O9W O6W Na6 78.2(2) . . ?
O9W O6W Na3 66.5(3) . 3_565 ?
Na6 O6W Na3 122.05(19) . 3_565 ?
O10W O8W Na4 95.9(9) . 3_565 ?
O10W O8W Na4 91.4(9) . . ?
Na4 O8W Na4 92.9(3) 3_565 . ?
O6W O9W Na3 70.4(2) . 3_565 ?
O6W O9W Na6 55.9(2) . . ?
Na3 O9W Na6 110.2(3) 3_565 . ?
O8W O10W N3 157.2(14) . . ?
O8W O10W Na4 67.7(8) . . ?
N3 O10W Na4 127.6(7) . . ?
O8W O10W Na4 63.6(8) . 3_565 ?
N3 O10W Na4 129.3(7) . 3_565 ?
Na4 O10W Na4 82.9(3) . 3_565 ?
O12W O11W Na5 90.2(10) . . ?
O12W O11W Na5 98.7(10) . 2_565 ?
Na5 O11W Na5 93.8(4) . 2_565 ?
O11W O12W N3 154.2(19) . . ?
O11W O12W Na5 68.9(8) . . ?
N3 O12W Na5 128.4(8) . . ?
O11W O12W Na5 61.7(9) . 2_565 ?
N3 O12W Na5 131.8(7) . 2_565 ?
Na5 O12W Na5 83.4(4) . 2_565 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.726(2) . ?
W1 O3 1.8599(18) . ?
W1 O2 1.8606(15) . ?
W1 O4 1.940(2) 2 ?
W1 O4 1.969(2) . ?
W1 O5 2.3500(16) . ?
W1 Na3 3.5756(10) 2 ?
W1 Na3 3.6808(10) . ?
W2 O6 1.723(2) . ?
W2 O7 1.792(2) . ?
W2 O8 1.9035(15) . ?
W2 O9 1.9514(14) . ?
W2 O3 2.0599(17) . ?
W2 O10 2.318(2) . ?
W2 Na3 3.4842(12) 2 ?
W3 O11 1.7238(18) . ?
W3 O12 1.797(2) . ?
W3 O8 1.9183(17) . ?
W3 O9 1.9452(19) 3 ?
W3 O2 2.0203(17) . ?
W3 O10 2.3627(14) 3 ?
W3 Na3 3.5090(12) . ?
Ni1 O13 2.012(3) . ?
Ni1 N1 2.042(6) 3 ?
Ni1 O7 2.035(2) 3 ?
Ni1 O13 2.037(2) 3 ?
Ni1 O12 2.048(2) . ?
Ni1 O14 2.0754(19) . ?
Ni1 N1 2.107(7) . ?
Ni1 O10 2.1972(19) 3 ?
Ni1 Ni2 2.9282(5) . ?
Ni1 Na4 3.414(2) . ?
Ni1 Na5 3.480(3) 3 ?
Ni2 O13 2.016(3) 3 ?
Ni2 O13 2.016(3) 2 ?
Ni2 O13 2.016(3) . ?
Ni2 O15 2.0486(19) . ?
Ni2 O15 2.0487(19) 3 ?
Ni2 O15 2.0489(19) 2 ?
Ni2 N1 2.143(8) 3 ?
Ni2 N1 2.144(8) . ?
Ni2 N1 2.144(8) 2 ?
Ni2 Ni1 2.9282(5) 3 ?
Ni2 Ni1 2.9283(5) 2 ?
Si1 O10 1.6248(19) 2 ?
Si1 O10 1.6249(19) 3 ?
Si1 O10 1.6249(19) . ?
Si1 O5 1.652(3) . ?
O1 Na3 2.334(2) 14_455 ?
O2 Na3 2.585(2) . ?
O3 Na3 2.4950(18) 2 ?
O4 W1 1.940(2) 3 ?
O4 Na3 2.8328(17) . ?
O5 W1 2.3500(16) 3 ?
O5 W1 2.3500(16) 2 ?
O6 Na1 2.296(2) 1_455 ?
O7 Ni1 2.035(2) 2 ?
O7 Na5 2.278(4) . ?
O9 W3 1.9452(19) 2 ?
O9 Na3 2.433(2) 2 ?
O10 Ni1 2.1971(19) 2 ?
O10 W3 2.3628(14) 2 ?
O11 Na6 2.382(4) . ?
O12 Na4 2.285(3) . ?
O13 N2 1.390(10) . ?
O13 Ni1 2.038(2) 2 ?
N1 N2 1.228(12) . ?
N1 Ni1 2.042(6) 2 ?
N2 N3 1.245(12) . ?
N3 O12W 1.359(17) . ?
N3 O10W 1.766(10) . ?
O14 C1 1.269(3) . ?
O14 Na4 2.566(3) . ?
O14 Na5 2.671(4) 3 ?
O15 C1 1.257(3) . ?
O15 Na2 2.3400(19) . ?
C1 C2 1.515(5) . ?
C2 H2A 0.9800 . ?
C2 H2B 0.9800 . ?
C2 H2C 0.9800 . ?
Na1 O6 2.296(2) 1_655 ?
Na1 O6 2.296(2) 3 ?
Na1 O6 2.296(2) 2_665 ?
Na1 O1W 2.361(2) 2_655 ?
Na1 O1W 2.361(2) . ?
Na1 O1W 2.361(2) 3_665 ?
Na1 Na3 4.0196(14) 2_655 ?
Na1 Na3 4.0197(14) 3_665 ?
Na1 Na3 4.0197(14) . ?
Na2 O15 2.3397(19) 3 ?
Na2 O15 2.3398(19) 11 ?
Na2 O15 2.3398(19) 10 ?
Na2 O15 2.3398(19) 12 ?
Na2 O15 2.3398(19) 2 ?
Na2 Ni2 2.9301(6) 10 ?
Na3 O1 2.334(2) 15 ?
Na3 O9W 2.413(6) 2_665 ?
Na3 O9 2.433(2) 3 ?
Na3 O6W 2.480(5) 2_665 ?
Na3 O3 2.4949(18) 3 ?
Na3 O1W 2.541(3) 3_665 ?
Na3 W2 3.4840(12) 3 ?
Na3 W1 3.5755(10) 3 ?
Na4 O8W 2.347(7) 2_665 ?
Na4 O8W 2.373(8) . ?
Na4 O2W 2.387(3) . ?
Na4 O5W 2.470(4) . ?
Na4 O10W 2.564(10) . ?
Na4 O10W 2.606(11) 2_665 ?
Na4 Na5 3.417(4) 3 ?
Na4 Na4 3.421(4) 2_665 ?
Na4 Na4 3.421(4) 3_565 ?
Na5 O4W 2.366(4) . ?
Na5 O11W 2.373(9) . ?
Na5 O11W 2.388(10) 3_455 ?
Na5 O5W 2.452(4) 2 ?
Na5 O12W 2.544(11) . ?
Na5 O14 2.671(4) 2 ?
Na5 O12W 2.680(12) 3_455 ?
Na5 Na4 3.417(4) 2 ?
Na5 Na5 3.477(5) 2_565 ?
Na5 Na5 3.477(5) 3_455 ?
Na5 Ni1 3.480(3) 2 ?
Na6 O6W 2.076(4) 2_665 ?
Na6 O6W 2.076(4) 3_565 ?
Na6 O6W 2.076(4) . ?
Na6 O11 2.382(4) 2_665 ?
Na6 O11 2.382(4) 3_565 ?
Na6 O9W 2.453(8) 2_665 ?
Na6 O9W 2.453(8) 3_565 ?
Na6 O9W 2.453(8) . ?
Na6 O3W 2.610(6) . ?
Na6 Na3 3.9905(18) 2_665 ?
O1W Na3 2.541(3) 2_655 ?
O2W Na4 2.387(3) 2_665 ?
O2W Na4 2.387(3) 3_565 ?
O3W Na6 2.610(6) 13_565 ?
O4W Na5 2.366(4) 2_565 ?
O4W Na5 2.366(4) 3_455 ?
O5W Na5 2.452(4) 3 ?
O6W O9W 1.799(7) . ?
O6W Na3 2.480(5) 3_565 ?
O8W O10W 0.917(10) . ?
O8W Na4 2.347(7) 3_565 ?
O9W Na3 2.413(6) 3_565 ?
O10W Na4 2.606(11) 3_565 ?
O11W O12W 0.907(18) . ?
O11W Na5 2.388(10) 2_565 ?
O12W Na5 2.680(12) 2_565 ?
